High-Pressure Shock Compression of Solids VI pp 57-119 | Cite as

# Paradigms and Challenges in Shock Wave Research

## Abstract

Shock compression science is a relatively new discipline that enables studies of materials in thermodynamic regimes inaccessible by other methods. The underlying motivation for these studies is to promote a physical understanding of dynamic material response. A fundamental understanding of material compression allows development of material models used to predict the response of materials subjected to dynamic loading. The past fifty years have produced a challenging research environment, resulting in the discovery and implementation of a broad spectrum of experimental, theoretical, and computational methods for this purpose. As a result, a large variety of phenomenological models have been developed for use in numerical simulations of material response under complex loading conditions. Even after a half-century of intensive research, however, there are still a large number of shock processes that cannot be resolved *a priori* with our existing level of understanding. A few examples include the prediction of shock transition times, compressive or tensile strengths under shock loading, and the kinetics of shock-induced phase transitions. This has led us to examine the issue of “what is a shock?” in tllis chapter by looking at the fundamental assumptions. These include assumptions of uniaxial displacement for applied planar loading, steady shock wave propagation, homogeneous shocked states, and thermodynamic equilibrium in tile shocked state. We examine the traditional approaches used for describing shock processes in solids, including the apparent anomalous observations resulting from these interpretations. Both experimental and computational results are used to show that shocks produce highly heterogeneous states of compression, which strongly influence observable material properties in the shocked state. Understanding these effects will require improved experimental diagnostics to probe deformation mechanisms *in situ* and in real time. We conclude by discussing what kinds of measurements will be needed to resolve these issues.

## Keywords

Shock Wave Shock Front Shock Compression Shock Propagation Shock Loading## Preview

Unable to display preview. Download preview PDF.

## References

- [1]Abou-Sayed, A.S., R.J. Clifton, and L. Herman (1976), “The oblique-plate impact experiment,”
*Exp. Mech*.**16**, pp. 127–132.Google Scholar - [2]Al’tshuler, L.V. (1978), “Phase transitions in shock waves (review),”
*J. Appl. Mech. Phys*.**18**, pp. 496–505.ADSGoogle Scholar - [3]Al’tshuler, L.V., M.N. Pavlovskii, V.V. Komissarov, and P.V. Makarov (1999), “Shear strength of aluminum in shock waves,”
*Combustion, Explosion and Shock Waves*,**35**, pp. 92–96.Google Scholar - [4]Ananin, A.V., O.N. Breusov, A.N. Dremin, S.V. Pershin, and V.F. Tatsii, (1974), “The effect of shock waves on silicon dioxide 1. quartz,”
*Combustion, Explosion, and Shock Waves***10**, p. 372.Google Scholar - [5]Atroshenko, S.A., and N.I. Zhigacheva (1996), “The method of visualization of dynamic deformation modes of metals,” in
*Shock Compression of Condensed Matter—1995*(eds. S.C. Schmidt and W.C. Tao), Amer. Inst. of Phys., NY.Google Scholar - [6]Asay, J.R., G.R. Fowles, G.E. Duvall, M.H. Miles and R.F. Tender (1972), “Effects of point defects on elastic precursor decay in LiF,”
*J. Appl. Phys.***43**, pp. 2132–2145.ADSGoogle Scholar - [7]Asay, J.R., D.L. Hicks, and D.B. Holdridge (1975), “Comparison of experimental and calculated elastic-plastic wave profiles in LiF,”
*J. Appl. Phys.***46**, pp. 4316–4322.ADSGoogle Scholar - [8]Asay, J.R. and L.M Barker (1974), “Interferometric measurement of shock-induced internal particle velocity and spatial variations of particle velocity,”
*J. Appl. Phys.***45**, pp. 2540–2546.ADSGoogle Scholar - [9]Asay, J.R., and L.C. Chhabildas (1980), “Shear strength of shock-loaded polycrystalline tungsten,”
*J. Appl. Phys*.**51**, pp. 4774–4783.ADSGoogle Scholar - [10]Asay, J.R. and L.C. Chhabildas (1981), “Determination of the shear strength of shock compressed 6061-T6 aluminum,” in
*Shock Waves and High-Strain-Rate Phenomena in Metals: Concepts and Applications*, (eds. Marc A. Meyers and Lawrence E. Murr), Plenum Publishing Corporation NY.Google Scholar - [11]Asay, J.R. and G.I. Kerley (1987), “The response of materials to dynamic loading,”
*Int'l. J. Impact Engineering***5**, pp. 66–99.Google Scholar - [12]Baer, M.R., M.E. Kipp, and F. van Swol (2001), “Microstructural mechanical modeling of heterogeneous energetic materials,” in: Proceedings of the Eleventh International Detonation Symposium, in press.Google Scholar
- [13]Baer, M.R. and W.M. Trott (2001), “Mesoscale descriptions of shock-loaded heterogeneous porous materials,”
*Bulletin of the Amer. Phys. Soc*.**46**, p. 102.Google Scholar - [14]Bancroft, D., E.L. Peterson, and S. Minshall (1956), “Polymorphism of Iron at High Pressure,”
*J. Appl. Phys*.,**27**, pp. 291–298.ADSGoogle Scholar - [15]Band, W. (1960), “Studies in the theory of shock propagation in solids,”
*J. Geophys. Res*.**65**, pp. 695–719.ADSGoogle Scholar - [16]Barker, L.M. (1968), “Fine Structure of Compressive and Release Wave Shapes in Aluminum Measured by the Velocity Interferometer Technique,” in:
*Behavior of Dense Media Under High Dynamic Pressures*, Gordon & Breach N.Y, p. 483.Google Scholar - [17]Barker, L.M. (1971), “A Model for Stress Wave Propagation in Composite Materials,”
*J. Composite Materials***5**, 140–162.ADSGoogle Scholar - [18]Barker, L.M., and R.E. Hollenbach (1974) “Shock wave study of the α ⇔ ε phase transition in iron,”
*J. Appl. Phys*.**45**(11), pp. 4872–4887.ADSGoogle Scholar - [19]Baumung, K., H.J. Bluhm, B. Goel, P. Hoppe, H.U. Karow, D. Rusch, V.E. Fortov, G.I. Kanel, A.V. Razorenov, A.V. Utkin, and O.Yu. Vorobjev (1986), in:
*Laser and Particle Beams*,**14**, Cambridge Univ. Press, pp. 181–209.Google Scholar - [20]Bishop, D., P. Gammel, and C.R. Giles (2001), “The little machines that are making it big,” in
*Physics Today***54**, pp. 38–44.Google Scholar - [21]Bland, D.R. (1964), “Dilatational waves and shocks in large displacement isentropic dynamic elasticity,”
*J. Mech. Phys.***12**, pp. 245–267.MathSciNetADSGoogle Scholar - [22]Bloomquist, D.D., and S.A. Sheffield (1983), “Optical recording interferometer for velocity measurements with subnanosecond resolution,”
*J. Appl. Phys*.**54**pp. 1717–1722.ADSGoogle Scholar - [23]Brannon, P.J, C. Konrad, R.W. Morris, E.D. Jones and J.R. Asay (1983), “Studies of the Spectral and Spatial Characteristics of Shock-Induced Luminescence from x-cut Quartz,”
*J. Appl. Phys*.**54**, pp. 6374–6381.ADSGoogle Scholar - [24]Briant, C., B. Morris, T. Tombrello, and S. Yip (2001) “Report on the Bodega Bay Workshop on Multi-Scale Modeling of Materials,” Oct. 7-10.Google Scholar
- [25]Bridgman, P.W. (1956), “High-pressure polymorphism of iron,”
*J. Appl. Phys*.**27**, p. 659.ADSGoogle Scholar - [26]Chhabildas, L.C. H.J. Sutherland, and J.R. Asay (1979), “A velocity interferometer teclmique to determine shear-wave particle velocity in shock-loaded solids,”
*J. Appl. Phys*.**50**, pp. 5196–5201.ADSGoogle Scholar - [27]Chhabildas, L.C., and J.R. Asay, (1979), “Rise-time measurements of shock transitions in aluminum, copper and steel,”
*J. Appl. Phys*.**50**, pp. 2749–2756.ADSGoogle Scholar - [28]Chhabildas, L.C., and J.R. Asay (1982), “Time-Resolved Wave Profile Measurements in Copper to Megabar Pressures,” in:
*High Pressure in Research and Industry***VI**(eds. C.M. Backman, T. Johanisson, and L. Tegner), pp. 183–189.Google Scholar - [29]Chhabildas, L.C., J.L. Wise, and J.R. Asay (1982), “Reshock and Release Behavior of Beryllium,” in:
*Shock-waves in Condensed Matter—1981*, (eds. W.J. Nellis, L. Seaman, and R.A. Graham, American Institute of Physics, New York, pp. 422–426.Google Scholar - [30]Chhabildas, L.C. and R.A. Graham (1987), in: Techniques and theory of stress measurements for shock wave applications,
*AMD***83**(eds. R.R. Stout, F.R. Norwood, and M.E. Fourney), ASME New York, pp. 1–18.Google Scholar - [31]Chhabildas, L.C., J.R. Asay, and L.M. Barker (1988)
*Shear Strength of Tungsten under Shock-and Quasi-Isentropic Loading to 250 GPa*, Sandia Report SAND88-0306 (unpublished).Google Scholar - [32]Chhabildas, L.C., W.M. Trott, and W.D. Reinhart (2001), “Incipient Spall Studies in Tantalum-Microstructural Effects,”
*Bulletin of the Amer. Phys. Soc*.**46**, p. 25.Google Scholar - [33]Conley, P.A., D.J. Benson, and P.M. Howe (2001), “Microstructural effects in shock initiation,” in: Proceedings of the Eleventh International Detonation Symposium, in press.Google Scholar
- [34]Courant, R., and K.O. Friedrichs (1948), Supersonic Flow and Shock Waves, Interscience, New York, 1991Google Scholar
- [35]Curran, D.R., L. Seaman, and D.A. Shockey (1987), “Dynamic Failure Of Solids,”
*Phys. Reports***147**, p. 253.ADSGoogle Scholar - [36]D’Almeida, T., and Y.M. Gupta (2000), “Real-time x-ray diffraction measurements of the phase transition in KCI shocked along [100],”
*Phys. Rev. Lett*.**85**, pp. 330–333.ADSGoogle Scholar - [37]Davis, J.P. (2001), “Formation of shocks from ramp input,” Sandia National Laboratories, private communication.Google Scholar
- [38]Davison, L. and R.A. Graham (1979), “Shock Compression of Solids,”
*Physics Reports***55**, pp. 257–379.ADSGoogle Scholar - [39]Davison, L. (2002), “Traditional analysis of nonlinear wave propagation in solids,” This volume, Chapter 1.Google Scholar
- [40]Divakov, A.K., L.S. Kokhanchik, Yu.I. Mescheryakov, and M.M. Myshlyaev (1987), “Micromechanics of dynamic deformation and failure,” Translated from Zhurnal
*Prikladnoi Mekhaniki i Tekhnicheskoi Fiziki*, pp. 135–144.Google Scholar - [41]Dremin, A.N., and O.N. Breusov (1968), “Processes Occurring in Solids Under the Action of Powerful Shock Waves,”
*Russian Chemical Reviews***37**, pp. 392–402.ADSGoogle Scholar - [42]Dhere, A.G., and M.A. Meyers (1982), “Correlation between texture and substructure of conventionally and shock-wave-deformed aluminum,”
*Materials Science and Engineering***54**, pp. 113–120.Google Scholar - [43]Dunn, J.E. (1990), “Implications and origins of shock structure in solids,” in:
*Shock Compression of Condensed Matter—1989*(eds. S.C. Schmidt, J.N. Johnson, and L.W. Davison), Elsevier Science Publishers B.V. Amsterdam, pp.21–32 (1990).Google Scholar - [44]Duvall, G.E., and G.R. Fowles (1963), “Shock Waves,”
*High Pressure Physics and Chemistry 2*, Chap. 9 (ed. R.S. Bradley), Academic Press New York.Google Scholar - [45]Duvall, G.E., and R.A. Graham (1977), “Phase transitions under shock-wave loading,”
*Rev. Modern Phys*.**49**, pp. 523–579.ADSGoogle Scholar - [46]Egorov, L.A., A.I. Barenboim, V.V. Mokhova, V.V. Dorohin, and A.I. Samoilov (1997), “X-ray diffraction studies of structures of Be, Al, LiF, Fe + 3%Si, Si, SiO
_{2}, KCl under dynamic pressures from 2 GPa to 20 GPa,”*Journal de Physique IV*,**7**(C3), pp. 355–360.Google Scholar - [47]Fowles, G.R. (1961), “Shock Wave Compression of Hardened and Annealed 2024 Aluminum,”
*J. Appl. Phys*.**32**, 1475–1487.ADSGoogle Scholar - [48]Fowles, G.R. (1972), “Experimental technique and Instrumentation,” in:
*Dynamic Response of Materials to Impulsive Loading*(eds. P.C. Chou and A.K. Hopkins), pp. 405–480.Google Scholar - [49]Gahagan, K.T., D.S. Moore, D.J. Funk, R.L. Rabie, S.J. Buelow, and J.W. Nicholson (2000), “Measurement of shock wave rise times in metal thin films,”
*Phys. Rev. Lett*.**85**, pp. 3205–3208.ADSGoogle Scholar - [50]Germann, T.C., B.L. Holian, P.S. Lomdahl (2000), “Orientation dependence of molecular dynamic simulations of shocked single crystals,”
*Phys. Rev. Lett*.**84**, pp. 5351–5354.ADSGoogle Scholar - [51]Gilman, J.J. (2001), “Elastic-plastic impact (some persistent mis-conceptions),” in:
*Fundamental Issues and Applications of Shock-Wave and High-Strain-Rate Phenomena*(eds. K.P. Staudhammer, L.E. Murr, and M.A. Meyers), Elsevier Sciences Ltd., New York.Google Scholar - [52]Gillman, J.J. (2001), private communication.Google Scholar
- [53]Grady, D.E., W.J. Murri, and P.S. DeCarli, (1975) “Hugoniot Sound Velocities and Phase Transformation in Two Silicates,”
*J. Geophys. Res*.**80**, p. 4857.ADSGoogle Scholar - [54]Grady, D.E. (1981), “Strain-rate dependence of the effective viscosity under steady-wave shock compression,”
*Appl. Phys. Lett*.**38**, pp. 825–827.ADSGoogle Scholar - [55]Grady, D.E. and J.R. Asay (1982), “Calculation of thermal trapping in shock deformation of aluminum,”
*J. Appl. Phys*.**53**, p. 7350.ADSGoogle Scholar - [56]Grady, D.E. (1998), “Scattering as a mechanism for structured shock waves in metals,”
*J. Mech. Solids***10**, pp. 2017–2032.ADSGoogle Scholar - [57]Graham, R.A. (1979). “Shock-induced electrical activity in polymeric solids. A mechanically induced bond scission model,”
*J. Phys. Chem*.**83**, pp. 3048–3056.Google Scholar - [58]Graham, R.A., and J.R. Asay (1978), “Measurements of wave profiles in shock-loaded solids,”
*High-Temperatures-High Pressures***10**, pp. 355–390.Google Scholar - [59]Graham, R.A. and D.M. Webb (1984), “Fixtures for Controlled Explosive Loading and Preservation of Powder Samples,” in:
*Shock-waves in Condensed Matter—1983*(eds. J.R. Asay, R.A. Graham, and G.K. Straub), Elsevier Science Publishers, Amsterdam, pp. 211–214.Google Scholar - [60]Graham, R.A. (1993a),
*Solids Under High-Pressure Shock Compression: Mechanics, Physics, and Chemistry*, Springer-Verlag, New York.Google Scholar - [61]Graham, R.A., (1993b), “Bridgman’s Concern,”
*High Pressure Science and Technology, Part 1*, (eds. S.C. Sdunidt, J.W. Shaner, G.A. Samara, and M. Ross), American Institute of Physics, New York, pp. 3–12.Google Scholar - [62]Gray, G.T. III (1993), “Influence of shock-wave deformation on the structure/property behavior of materials,” in
*High-Pressure Shock Compression of Solids*(eds. J.R. Asay and M. Shahinpoor), Springer-Verlag, New York, pp. 187–213.Google Scholar - [63]Guduru, P.R., A.J. Rosakis, and G. Ravichandran (2001a), “Dynamic shear bands: an investigation using high speed optical and infrared diagnostics,”
*Mech. of Materials***33**, pp. 371–402.Google Scholar - [64]Guduru, P.R., A.T. Zehnder, A.J. Rosakis, and G. Ravichandran (2001b), “Dynamic full field measurements of crack tip temperatures,”
*Eng. Frac. Mech*.**68**, pp. 1535–1556.Google Scholar - [65]Gupta, Y.M. (1975), “Stress dependence of elastic-wave attenuation in LiF,”
*J. Appl. Phys*.**46**, pp. 3395–3401.ADSGoogle Scholar - [66]Gupta, Y.M. (1977), “Effect of crystal orientation on dynamic strength of LiF,”
*J. Appl. Phys*.**48**, pp. 5067–5073.ADSGoogle Scholar - [67]Gupta, Y.M., D.D. Keough, D. Henley, and D.F. Walter (1980), “Measurement of lateral compressive stresses under shock loading,”
*Appl. Phys. Lett*.**37**, pp. 395–397.ADSGoogle Scholar - [68]Gupta, Y.M., K.A. Zimmerman, P.A. Rigg, E.B. Zaretsky, D.M. Savage, and P.M. Bellamy (1999), “Experimental developments to obtain real-time x-ray diffraction measurements in plate impact experiments,”
*Rev. Sci. Instr*.**10**, pp. 4008–4014.ADSGoogle Scholar - [69]Gupta, Y.M. (2000) “Shock wave experiments at different length scales: recent achievements and future challenges,”
*Shock Compression of Condensed Matter—1999*, (eds. M.D. Furnish, L.C. Chhabildas, and R.A. Hixson), Amer. Inst. Phys., pp. 3–10.Google Scholar - [70]Hare, D. (2001), “Optical emission of sapphire shock-loaded to 255 GPa,”
*Bulletin of the Amer. Phys. Soc*.**46**, p. 22.Google Scholar - [71]Herrmann, W. (1974), “Development of a high strain rate constitutive equation for 6061-T6 aluminum,” Sandia National Laboratories Report SLA-73 0897, unpublished.Google Scholar
- [72]
- [73]Hodowany, J.G. Ravichandran, A.J. Rosakis and P. Rosakis (1998), “On the partition of plastic work into heat and stored energy in metals; part I: Experiments,” California Institute of Technology Report SM Report 98-7.Google Scholar
- [74]Holian, B.L., and G.K. Straub (1979), “Molecular dynamics of shock waves in three-dimensional solids: transition from non steady to steady waves in perfect crystals and implication for the Rankine-Hugoniot conditions,”
*Phys. Rev. Lett*.**43**, pp. 1598–1600.ADSGoogle Scholar - [75]Holian, B.L. and G.K. Straub (1980), “Shock-wave structure via nonequilibrium molecular dynamics and Navier-Stokes continuum mechanics,”
*Phys. Rev. A***22**, pp. 2798–2808.ADSGoogle Scholar - [76]Holian, B.L. (1988), “Modeling shock-wave deformation via molecular dynamics,”
*Phys. Rev. A***37**, pp. 2562–2568.ADSGoogle Scholar - [77]Holian, B.L. (1995), “Atomistic computer simulations of shock waves,”
*Shock Waves***5**, pp. 149–157.ADSGoogle Scholar - [78]
- [79]Holian, B.L. (2002), “What is a shock wave?—The view from the atomic scale,” this volume, Chap. 4.Google Scholar
- [80]Hoover, W.G. (1979), “Structure of a shock wave in a liquid,”
*Phys. Rev. Lett*.**42**, pp. 1531–1534.ADSGoogle Scholar - [81]Horie, Y. (1970a), “Characteristics of compressible fluids and the effects of heat conduction and viscosity,”
*Amer. J. Phys*.**38**, pp. 212–215.ADSGoogle Scholar - [82]Horie, Y. (1970b), “An aspect of energy transfer in axial impact of rods,” TR 70-6, North Carolina State University, September 1970, Raleigh, NC, prepared for ONR under contract N00014-68-A-0187.Google Scholar
- [83]Horie, Y. (1971), “Adiabatic theory of plane steady shock profiles in solids,”
*J. Appl. Phys*.**42**, pp. 2925–2933.ADSGoogle Scholar - [84]Horie, Y. and H.L. Chang (1972), “Analysis of plane shock structures in 6061-T6 aluminum,”
*J. Appl. Phys*.**43**, pp. 3362–3368.ADSGoogle Scholar - [85]Horie, Y. (1973), “Classification of steady-profile shocks in liquids,”
*J. Appl. Phys*.**45**, pp. 759–764.ADSGoogle Scholar - [86]Horie, Y. (1976), “Thermal-energy relaxation in shock-compressed solids,”
*J. Mech. Phys. Solids***24**, pp. 361–379.ADSGoogle Scholar - [87]Hugoniot, P.H. (1889), “On the propagation of movement in bodies, in particular in ideal gases,”
*J. de l'Ecole Polytechnique***57**.Google Scholar - [88]Johnson, J.N. (1993), “Micromechanical considerations in shock compression of solids,” in
*High-Pressure Shock Compression of Solids*(eds. J.R. Asay and M. Shahinpoor) Springer-Verlag, New York, pp. 222–240.Google Scholar - [89]Johnson, J.N. and L.M. Barker (1969), “Dislocation dynamics and steady plastic wave profiles in 6061-T6 aluminum,”
*J. Appl. Phys*.**40**, pp. 4321–4334.ADSGoogle Scholar - [90]Johnson, J.N., O.E. Jones, and T.E. Michaels (1970), “Dislocation dynamics and single-crystal constitutive relations: shock-wave propagation and precursor decay,”
*J. Appl. Phys*.**41**, pp. 2330–2339.ADSGoogle Scholar - [91]Johnson J.N., R.S. Hixson, and G.T. Gray III (1994), “Shock-wave compression and release of aluminum/ceramic composites,”
*J. Appl. Phys*.**76**, pp. 5706–5718.ADSGoogle Scholar - [92]Johnson, Q., A. Mitchell, R.N. Norris, and L. Evans (1970), “X-ray diffraction during shock-wave compression,”
*Phys. Rev. Lett*.**25**, pp. 1099–1101.ADSGoogle Scholar - [93]Johnson, Q., and A.C. Mitchell (1972), “First x-ray diffraction evidence for a phase transition during shock-wave loading,”
*Phys. Rev. Lett*.**29**, p. 1369.ADSGoogle Scholar - [94]Jones, O.E., and J.D. Mote (1969), “Shock-induced dynamic yielding in copper single crystals,”
*J. Appl. Phys*.**40**, pp. 4920–4928.ADSGoogle Scholar - [95]Kadau, K., T.C. Germann, P.S. Lomdahl, and B.L. Holian (2002), “Microscopic view of structural phase transitions due to shock waves,” submitted to Science.Google Scholar
- [96]Kalantar, D.H., B.A. Remington, J.D. Colvin, K.O. Mikaelian, S.V. Weber, L.G. Wiley, J.W. Wark, A. Loveridge, A.M. Allen, A.A. Hauer, and M.A. Meyer (2000), “Solid-state experiments at high pressure and strain rate,”
*Phys. Plasmas***7**, pp. 1999–2006.ADSGoogle Scholar - [97]Kerley, G.I. (2000), “XRB: A new reactive burn model for heterogeneous and homogenous explosives,” Kerley Publishing Co. Report KPS00-1.Google Scholar
- [98]Kanel, G.I., G.E. Vakhitova, and A.N. Dremin, (1978), “Metrological characteristics of manganin pressure pickups under conditions of shock compression and unloading,”
*Combustion, Explosion, and Shock Waves***14**, pp. 244–248.Google Scholar - [99]Kanel, G.I., M.F. Ivanov, and A.N. Parshikov (1995), “Computer simulation of the heterogeneous materials response to the impact loading,”
*Int. J. Impact. Eng*.**17**, pp. 455–464.Google Scholar - [100]Khantuleva, T.A. (2000), “Non-local theory of high-rate straining followed by structure formations,”
*J. Phys. IV, France***10**, 485–490.Google Scholar - [101]Khantuleva, T.A, and Yu.I. Meshcheryakov (1999), “Non-local theory of the high-strain-rate processes in structured media,”
*International J. Solids and Stroctures***36**, pp. 3105–3129.zbMATHGoogle Scholar - [102]Knudson, M.D. (1999), “Transformation mechanism for the pressure-induced phase transition in shocked CdS,”
*Phys. Rev. B***59**, pp. 11704–11715.ADSGoogle Scholar - [103]Knudson, M.D. and Y.M. Gupta (2002), “Transformation kinetics for the shock wave induced phase transition in cadmium sulfide crystals,” submitted to
*Phys. Rev. Lett*.Google Scholar - [104]Kim, K.S., R.J. Clifton, and P. Kumar (1977), “A combined normal-and transverse-displacement interferometer with an application to impact of y-cut quartz,”
*J. Appl. Phys*.,**48**, pp. 4132–4139.ADSGoogle Scholar - [105]Kumar, P. and R.J. Clifton (1977), “Star-shaped flyer for plate-impact recovery experiments,”
*J. Appl. Phys*.**48**, pp. 4850–4852.ADSGoogle Scholar - [106]Kipp, M.E., L.C. Chhabildas, W.D. Reinhart, and M.K. Wong (2000), “Polyurethane foam impact experiments and simulations,” in:
*Shock Waves in Condensed Matter—1999*(eds. M.D. Furnish, L.C. Chhabildas, and R.S. Hixson), American Institute of Physics, New York, pp. 313–316.Google Scholar - [107]Kormer, S.B. (1968), “Optical study of the characteristics of shock-compressed condensed dielectrics,”
*Sov. Phys. Uspekhi***11**, pp. 229–254.ADSGoogle Scholar - [108]Larsson, J., Z. Chang, E. Judd, P.J. Schuck, R.W. Falcone, P.A. Heimann, H.A. Padmore, H.C. Kapteyn, P.H. Bucksbaum, M.N. Murnane, R.W. Lee, A. Machacek, J.S. Wark, X. Liu, and B. Shan (1997), “Ultrafast x-ray diffraction using a streak camera detector in averaging mode,”
*Optics Letters***22**, pp. 1012–1014.ADSGoogle Scholar - [109]Larsson, J., P.A. Heimann, A.M. Lindenberg, P.J. Schuck, P.H. Bucksbaum, R.W. Lee, H.A. Padmore, J.S. Wark, and R.W. Falcone (1998), “Ultrafast structural changes measured by time-resolved x-ray diffraction,”
*Appl. Phys. A***66**, pp. 587–591.ADSGoogle Scholar - [110]Lindenberg, A.M, I. Kang, S.L. Johnson, T. Missalla, P.A. Heimann, Z. Chang, J. Larsson, P.H. Bucksbaum, H.C. Kapteyn, H.A. Padmore, R.W. Lee, J.S. Wark, and P.W. Falcone (2000), “Time-resolved x-ray diffraction from coherent phonons during a laser-induced phase transition,”
*Phys. Rev. Lett*.**84**, pp. 111–114.ADSGoogle Scholar - [111]Lipkin, J. and J.R. Asay (1977), “Reshock and release of shock-compressed 6061-T6 aluminum,”
*J. Appl. Phys*.**48**, p. 182.ADSGoogle Scholar - [112]Makarov, P.V. (1992) “Microdynamic theory of plasticity and failure of structurally inhomogeneous media,” Translated from
*Izvestiya Vysshikh Uchebnykh Zavedenii, Fizika***4**, pp. 42–58.Google Scholar - [113]Makarov, P.V. (1998), “Physical mesomechanics approach in simulation of deformation and fracture processes,”
*Physical Mesomechanics***1**, pp. 57–75.Google Scholar - [114]Mashimo, T., and M. Uchino (1997), “Heterogeneous free-surface profile of B
_{4}C polycrystal under shock compression,”*J. Appl. Phys*.**81**, pp. 7064–7066.ADSGoogle Scholar - [115]McQueen, R.G., S.P. Marsh, J.W. Taylor, J.N. Fritz and W.J. Carter (1970), “The equation of state of solids from shock wave studies,” in:
*High-Velocity Impact Phenomena*(ed. Ray Kinslow), Academic Press, New York, pp. 293–417.Google Scholar - [116]Meshcheryakov, Yu.I. (1983), “Relaxation of submicrosecond pressure pulses in a solid,” Translated from
*Zhurnal Prikladnoi Mekhaniki i Tekhnicheskoi Fiziki*,**2**, pp. 102–109.Google Scholar - [117]Meshcheryakov, Yu.I., and A.K. Divakov (1985), “Particle velocity variations in a shock wave and fracture strength of aluminum,”
*Sov. Phys. Tech. Phys*.**30**, pp. 348–350.Google Scholar - [118]Meshcheryakov, Yu., S.A. Atroshenko, V.B. Vasilkov and A.I. Chernyshenko (1992), “Criteria of transition from translation to rotational motion of media under shock loading,” in:
*Shock Compression of Condensed Matter—1991*(eds. S.C. Schmidt, R.D. Dick, J.W. Forbes and D.G. Tasker), Elsevier Sciences Publ., Amsterdam, pp. 407–441.Google Scholar - [119]Meshcheryakov, Yu.I., and S.A. Atroshenko (1992), “Dynamic rotations in crystals,” Translated from
*Izvestiya Vysshikh Uchebnykh Zavendenii, Fizika***4**, pp. 105–123.Google Scholar - [120]Meshcheryakov, Yu.I., N.A. Mahutov, and S.A. Atroshenko (1994), “Micromechanisms of dynamic fracture of ductile high-strength steel,”
*J. Mech. Phys. Solids***42**, pp. 1435–1457.ADSGoogle Scholar - [121]Meshcheryakov, Yu.I., and A.K. Divakov (1994), “Multi-scale kinetics of microstructure and strain-rate dependence of materials,”
*DYMAT Journal***1**, 271–287.Google Scholar - [122]Meshcheryakov, Yu., and S.A. Atroshenko (1995), “Dynamic recrystallization in shear bands,” in:
*Metallurgical and Materials Applications of Shock-Wave and High-Strain-Rate Phenomena*(eds. L.E. Murr, K.P. Staudhammer and M.A. Meyers), Elsevier Science B.V., Amsterdam.Google Scholar - [123]Meyers, M.A. (1975a), “A “wavy wave” model for the shocking of polycrystalline metals,” in:
*Proc. 5*^{th}*International Conf. On High-Energy Rate Fabrication*, Denver Research Institute, June.Google Scholar - [124]Meyers, M.A., (1975b), “The effect of surface conditions on shock hardening,”
*Scripta Metallurgica***9**, pp. 667–669.Google Scholar - [125]Meyers, M.A. and M.S. Carvalho, (1976), “Shock-front irregularities in polycrystalline metals,”
*Mat. Sci. and Eng*.**24**, pp. 131–135.Google Scholar - [126]Meyers, M.A. (1977), “A model for elastic precursor waves in the shock loading of polycrystalline metals,”
*Materials Science and Engineering*, pp. 99–111.Google Scholar - [127]Meyers, M.A., L.E. Murr, C.Y. Hsu, and G.A. Stone (1983), “The effect of polycrystallinity on the shock wave response of Fe-34.5wt.%Ni and Fe-15wt%Cr-15wt.%Ni,”
*Materials Science and Engineering***57**, pp. 113–126.Google Scholar - [128]Meyers, M.A., K.-C. Hsu, and K. Couch-Robino (1983), “The attenuation of shock waves in nickel: second report,”
*Materials Sci. and Engineering***59**, pp. 235–249.Google Scholar - [129]Mogilevsky, M.A. (1981), “Mechanisms of deformation under shock loading,” in:
*Shock Waves and High-Strain-Rate Phenomena in Metals: Concepts and Applications*(eds. Marc. A. Meyers and Lawrence E. Murr), Plenum Press, New York, pp. 531–546.Google Scholar - [130]Moore, D.S., K.T. Gahagan, J.H. Reho, D.J. Funk, S.J. Buelow, and R.L. Rabie (2001), “Ultrafast nonlinear optical method for generation of planar shocks,”
*Appl. Phys. Lett*.**78**, pp. 40–42.ADSGoogle Scholar - [131]Murri, W. (1974),
*Advances in High-Pressure Research, 4*(ed. R.H. Wentorf, Jr.), Academic Press, London and NY.Google Scholar - [132]Nesterenko, V.F. (2002),
*Dynamics of Heterogeneous Materials*, Springer-Verlag, New York, 2001.Google Scholar - [133]Nunziato, J.W., E.K. Walsh, K.W. Schuler, and L.M. Barker (1974), “Wave Propagation in Nonlinear Viscoelastic Solids,” in:
*Handbuch der Physik*, Vol. VIa/4, (ed. S. Flügge), Springer-Verlag, Berlin, pp. 1–108.Google Scholar - [134]Panin, V., Yu. V. Grinyaev, T.F. Elsukova, and A.G. Ivanehin (1982), “Structural levels of deformation in solids,”
*Izvestiya Vysshikh Uchebnykh Zavedenii, Fizika*,**6**, pp. 5–27.Google Scholar - [135]Panin, V.E. (1997), “Physical mechanisms of mesomechanics of plastic deformation and fracture of solids,”
*Acta Metallurgica Sinica***33**, pp. 187–197.Google Scholar - [136]Panin, V.E. (1998), “Foundations of physical mesomechanics,”
*Physical Mesomechanics***1**, pp. 5–20.Google Scholar - [137]Perry, F.C., and D.D. Noack (1986), “Heterogeneous response of aluminum and lithium niobate to shock waves,”
*Shock Waves in Condensed Matter*(ed. Y.M. Guptah), Plenum Press, New York, pp. 655–660.Google Scholar - [138]Persson, Per-Anders and Gunnar Persson (1972), “High-resolution photography of transverse wave effects in the detonation of condensed explosives,”
*Proceedings of 6*^{th}*Symposium on Detonation*, (ed. D.J. Edwards), Office of Naval Research, Arlington, VA. pp. 414–425.Google Scholar - [139]Reinhart, W.D., L.C. Chhabildas, D.E. Grady, and T. Mashimo (2002), “Shock compression and release properties of Coors AD995 alumina,” to be published in the proceedings of the American Ceramic Society PACRIM-Conference, November 3-6, 2001.Google Scholar
- [140]Rosakis, P., A.J. Rosakis, G. Ravichandran, and J. Hodowany (1998), “On the partition of plastic work into heat and stored energy in metals; Part II: Theory,” California Institute of Technology Report SM Report 98-8.Google Scholar
- [141]Rosenberg, Z. and Y. Partom (1985), “Lateral stress measurement in shock-loaded targets with transverse piezoresistance gauges,”
*J. Appl. Phys*.**58**, pp. 3072–3076.ADSGoogle Scholar - [142]Rice, M.H., R.G. McQueen and J.M. Walsh (1958), “Compression of solids by strong shock waves,” in:
*Solid State Physics***1**(eds. F. Seitz and D. Turnbull), Academic, New York, pp. 1–63.Google Scholar - [143]Rigg, P.A., and Y.M. Gupta (1998), “Real-time x-ray diffraction to examine elastic-plastic deformation in shocked lithium fluoride crystals,”
*J. Appl. Phys. Lett*.**73**, pp. 1655–1657.ADSGoogle Scholar - [144]Rigg, P.A. and Y.M. Gupta (2001), “Multiple x-ray diffraction to determine transverse and longitudinal lattice deformation in shocked lithium fluoride,”
*Phys. Rev B***63**, p. 094112.ADSGoogle Scholar - [145]Savenko, G.G., Yu.I. Mescheryakov, V.B. Vasil’kov and A.I. Chernyshenko (1990), “Grain vibrations and development of the turbulent nature of plastic deformation during high-velocity interaction of solid bodies,” Translated from
*Fizika Goreniya I Vzryva*,**26**, pp. 97–102.Google Scholar - [146]Swan, G.W, G.E. Duvall and C.K. Thornhill (1973), “On steady wave profiles in solids,”
*J. Mech. Phys. Solids***21**, pp. 215–227.ADSzbMATHGoogle Scholar - [147]Swegle, J.W., and D.E. Grady (1985), “Shock viscosity and the predictions of shock wave risetimes,”
*J. Appl. Phys*.**58**, pp. 692–701.ADSGoogle Scholar - [148]Swegle, J.W. and D.E. Grady (1986), “Calculation of thermal trapping in shear bands,” in:
*Metallurgical applications of shock-wave and high-strain-rate phenomena*, (eds. Lawrence E. Murr, Karl P. Staudhammer, and Marc A. Meyers), NY.Google Scholar - [149]Taylor, J.W. (1965), “Dislocation dynamics and dynamic yielding,”
*J. Appl. Phys*.**36**, pp. 3146–3150.ADSGoogle Scholar - [150]Taylor, J.W. (1984), “Thunder in the mountains,” in:
*Shock Waves in Condensed Matter—1983*(eds. J.R. Asay, R.A. Graham, and G.K. Straub), North-Holland, New York, pp. 3–15.Google Scholar - [151]Teller, E. (1962), “On the speed of reactions at high pressures,”
*J. Chem. Phys*.**36**, pp. 901–903.ADSGoogle Scholar - [152]Tomlin, M.G., Yu.I. Meshcheryakov, S.A. Atroshenko, N.I. Zhigacheva, and S.I. Vavilov (1994), “LC vision: the dynamically induced structure of deformation modes in metals,”
*Mol. Cryst. Liq. Cryst*.**251**, pp. 343–349.Google Scholar - [153]Trott, W.M, J.N. Castaneda, J.J. O'Hare, M.R. Baer, L.C. Chhabildas, M.D. Knudson, J.P. Davis, and J.R. Asay (2000), “Examination of the mesoscopic scale response of shock compressed heterogeneous materials using a line-imaging velocity interferometer,” in:
*Shock-Wave and High-Strain-Rate Phenomena*, (eds. K.P. Staudhammer, L.E. Murr, and M.A. Meyers), pp. 647–654.Google Scholar - [154]Trott, W.M., J.N. Castaneda, J.J. O'Hare, M.R. Baer, L.C. Chhabildas, M.D. Knudson, J.P. Davis, and J.R. Asay (2000), “Dispersive velocity measurements in heterogeneous materials,” Sandia National Laboratories report SAND2000-3082.Google Scholar
- [155]Trott, W.M., L.C. Chhabildas, M.R. Baer, J.N. Castaneda, J.J. O'Hare (2001), “Investigation of dispersive waves in low-density sugar and HMX using line-imaging velocity interferometry,”
*Bulletin of the Amer. Phys. Soc*.**46**, p. 31.Google Scholar - [156]Tonks, D.L. (1988), “Relation between shock strength and strain-rate plasticity at maximum deviatoric stress,”
*Shock Waves in Condensed Matter—1987*, (eds. S.C. Schmidt and N.C. Holmes), Elsevier Science Publishers B.V., Amsterdam.Google Scholar - [157]Urtiew, P.A. and A.K. Oppenheim (1966), “Experimental observations of the transition to detonation in an explosive gas,”
*Proc. Royal Soc*.**295**, pp. 13–28.ADSGoogle Scholar - [158]Urtiew, P.A. (1970), “Reflections of wave interactions in marginal detonations,”
*Astronautica Acta***15**, pp. 335–343.Google Scholar - [159]Urtiew, P.A. and A.S. Kusubov (1970), “Wall traces of detonation in nitromethane-acetone mixtures,” presented at the 5
^{th}Symposium on Detonation, Pasadena, CA, Aug. 18-21.Google Scholar - [160]Urtiew, P.A., A.S. Kusubov, and R.E. Duff (1970), “Cellular structure of detonation in nitromethane,”
*Combustion and Flame***14**, pp. 117–122.Google Scholar - [161]Urtiew, P.A. (1975), “From cellular structure to failure waves in liquid detonations,”
*Combustion and Flames***25**, pp. 241–245.Google Scholar - [162]Urtiew, P.A. (1976), “Idealized two-dimensional detonation waves in gaseous mixtures,”
*Acta Astronautica***3**, pp. 187–200.ADSGoogle Scholar - [163]Urtiew, P.A. and C.M. Tarver (1981), “Effects of cellular structure on the behavior of gaseous detonation waves under transient conditions,” in
*Gasdynamics of Detonations and Explosions*(eds. J.R. Bowen, N. Manson, A.K. Oppenheim, and R.I. Soloukhin), in: Progress in Astronautics and Aeronautics Vol. 75.Google Scholar - [164]Yano, K. and Y. Horie (1999), “Discrete-element modeling of shock compression of polycrystalline copper,”
*Phys. Rev. B***59**, p. 13672.ADSGoogle Scholar - [165]Yano, K., and Y. Horie (2002), “Mesomechanics of the (α-ε transition in iron,” submitted to
*Int. Journal of Plasticity*.Google Scholar - [166]Wallace, D.C. (1980a), “Flow processes of weak shocks in solids,”
*Phys. Rev. B*,**22**, pp. 1495–1502.MathSciNetADSGoogle Scholar - [167]Wallace, D.C. (1980b), “Irreversible thermodynamics of flow in solids,”
*Phys. Rev. B***22**, pp. 1477–1486.MathSciNetADSGoogle Scholar - [168]Wallace, D.C. (1981), “Irreversible thermodynamics of overdriven shocks in solids,”
*Phys. Rev. B***24**, pp. 5597–5606.ADSGoogle Scholar - [169]Wark, J.W. (1996), “Time-resolved X-ray diffraction,”
*Contemp. Phys*. (UK),**36**, pp. 205–218.ADSGoogle Scholar - [170]Whitlock, R.R, and J.S. Wark (1995), “Orthogonal strains and onset of plasticity in shocked LiF crystals,”
*Phys. Rev. B***52**, pp. 8–11.ADSGoogle Scholar - [171]Widmann, K., G. Guethlein, M.E. Foord, R.C. Cauble, F.G. Patterson, D.F. Price, F.J. Rogers, P.T. Springer, and R.E. Stewart (2001), “Interferometric investigation of femto-second laser-heated expanded states,”
*Physics of Plasmas***8**, pp. 3869–3872.ADSGoogle Scholar - [172]Zel’dovich, Ya.B., and Yu.P. Raizer (1966),
*Physics of Shock Waves and High-Temperature Hydrodynamic Phenomena*,**1**(eds. W.D. Hayes and R.F. Probstein) Academic Press, New York and London.Google Scholar - [173]Zaretskii, E.B., G.I. Kanel, P.A. Mogilevskii, and V.E. Fortov (1991), “Device for investigating x-ray diffraction on shock-compressed material,” translated from
*Teplofixika Vysokikh Temperatur***29**, pp. 1002–1008.Google Scholar - [174]Zaretskii, E.B., G.I. Kanel, P.A. Mogilevskii, and V.E. Fortov (1991), “X-ray diffraction study of phase transition mechanism in shock-compressed KCI single crystal,”
*Sov. Phys. Dokl*.**36**, pp. 76–78.ADSGoogle Scholar